English: Table II - Mark-up <TAB CO=7 ID=‘TABLE 1’ RS=‘PS FS AS’ CS=‘PS FS AS’> <ROW><TTI>THE CURING OF COATING COMPOSITIONS UNDER ULTRAVIOLET LIGHT <ROW><TCH><U>COMPOSITION</U> <TCH><U>TIME(MIN.)</U> <TCH>D-IMPACT<FOR FNREF="18.1">*</FOR><U>THICKNESS (MIL)</U> <TCH>R-IMPACT<FOR FNREF="18.2">**</FOR><U>ADHESION</U> <TCH><U>HARDNESS</U> <TCH><U>(IN-LB)<FOR FNREF="18.3">***</FOR></U> <TCH><U>(IN-LB2)<FOR FNREF="18.3">***</FOR></U> <ROW><TSB RB=3 RE=5>1<CEL>75<CEL AL=C>0.1-0.2<CEL>90 percent<CEL>8H<CEL>25<CEL>10 <ROW><CEL>180<CEL AL=C>0.3-0.5<CEL>100 percent<CEL>2H<CEL>50<CEL>10 <ROW><CEL>180<CEL>0.5<CEL>100 percent<CEL>HB<CEL>100<CEL>0 <ROW><TSB RB=6 RE=7>2<CEL>130<CEL AL=C>0.1-0.2<CEL>100 percent<CEL>8H<CEL>25<CEL>0 <ROW><CEL>150<CEL AL=C>0.1-0.2<CEL>100 percent<CEL>8H<CEL>25<CEL>0 <ROW><TSB RB=8 RE=9>3<CEL>60<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>50<CEL>0 <ROW><CEL>120<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>50<CEL>0 <ROW><TSB RB=10 RE=11>4<CEL>60<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>30<CEL>10 <ROW><CEL>90<CEL AL=C>1.0<CEL>60 percent<CEL>8H<CEL>40<CEL>10 <ROW><TSB RB=12>5<CEL>120<CEL AL=C>0.4-0.5<CEL>95 percent<CEL>8H<CEL>30<CEL>10 <ROW><TSB RB=13>6<CEL>120<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>25<CEL>0 <ROW><TSB RB=14 RE=15>7<CEL>60<CEL>0.4<CEL>100 percent<CEL>8H<CEL>160<CEL>50 <ROW><CEL>120<CEL AL=C>0.4<CEL>100 percent<CEL>8H<CEL>160<CEL>50 <ROW><TSB RB=16>8<CEL>60<CEL AL=C>0.4-0.5<CEL>100 percent<CEL>8H<CEL>75<CEL>10 <ROW><TSB RB=17>9<CEL>60<CEL AL=C>0.2-0.4<CEL>100 percent<CEL>8H<CEL>40<CEL>0 <ROW><TSB RB=18>10<CEL>60<CEL AL=C>0.2-0.4<CEL>100 percent<CEL>8H<CEL>40<CEL>0 <ROW><TSB RB=19>11<CEL>30<CEL AL=C>0.5<CEL>100 percent<CEL>8H<CEL>100<CEL>100 <ROW><TSB RB=20>12<CEL>30<CEL AL=C>0.05-0.07<CEL>100 percent<CEL>6H<CEL>40<CEL>10 <FOO FN="18.1">* Direct Impact</FOO> <FOO FN="18.2">** Reverse Impact</FOO> <FOO FN="18.3">*** Inch-Pounds</FOO> </TAB> Note:
French: Tableau II - Balisage <TAB CO=7 ID=‘TABLE 1’ RS=‘PS FS AS’ CS=‘PS FS AS’> <ROW><TTI>THE CURING OF COATING COMPOSITIONS UNDER ULTRAVIOLET LIGHT <ROW><TCH><U>COMPOSITION</U> <TCH><U>TIME(MIN.)</U> <TCH>D-IMPACT<FOR FNREF="18.1">*</FOR><U>THICKNESS (MIL)</U> <TCH>R-IMPACT<FOR FNREF="18.2">**</FOR><U>ADHESION</U> <TCH><U>HARDNESS</U> <TCH><U>(IN-LB)<FOR FNREF="18.3">***</FOR></U> <TCH><U>(IN-LB2)<FOR FNREF="18.3">***</FOR></U> <ROW><TSB RB=3 RE=5>1<CEL>75<CEL AL=C>0.1-0.2<CEL>90 percent<CEL>8H<CEL>25<CEL>10 <ROW><CEL>180<CEL AL=C>0.3-0.5<CEL>100 percent<CEL>2H<CEL>50<CEL>10 <ROW><CEL>180<CEL>0.5<CEL>100 percent<CEL>HB<CEL>100<CEL>0 <ROW><TSB RB=6 RE=7>2<CEL>130<CEL AL=C>0.1-0.2<CEL>100 percent<CEL>8H<CEL>25<CEL>0 <ROW><CEL>150<CEL AL=C>0.1-0.2<CEL>100 percent<CEL>8H<CEL>25<CEL>0 <ROW><TSB RB=8 RE=9>3<CEL>60<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>50<CEL>0 <ROW><CEL>120<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>50<CEL>0 <ROW><TSB RB=10 RE=11>4<CEL>60<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>30<CEL>10 <ROW><CEL>90<CEL AL=C>1.0<CEL>60 percent<CEL>8H<CEL>40<CEL>10 <ROW><TSB RB=12>5<CEL>120<CEL AL=C>0.4-0.5<CEL>95 percent<CEL>8H<CEL>30<CEL>10 <ROW><TSB RB=13>6<CEL>120<CEL AL=C>0.2<CEL>100 percent<CEL>8H<CEL>25<CEL>0 <ROW><TSB RB=14 RE=15>7<CEL>60<CEL>0.4<CEL>100 percent<CEL>8H<CEL>160<CEL>50 <ROW><CEL>120<CEL AL=C>0.4<CEL>100 percent<CEL>8H<CEL>160<CEL>50 <ROW><TSB RB=16>8<CEL>60<CEL AL=C>0.4-0.5<CEL>100 percent<CEL>8H<CEL>75<CEL>10 <ROW><TSB RB=17>9<CEL>60<CEL AL=C>0.2-0.4<CEL>100 percent<CEL>8H<CEL>40<CEL>0 <ROW><TSB RB=18>10<CEL>60<CEL AL=C>0.2-0.4<CEL>100 percent<CEL>8H<CEL>40<CEL>0 <ROW><TSB RB=19>11<CEL>30<CEL AL=C>0.5<CEL>100 percent<CEL>8H<CEL>100<CEL>100 <ROW><TSB RB=20>12<CEL>30<CEL AL=C>0.05-0.07<CEL>100 percent<CEL>6H<CEL>40<CEL>10 <FOO FN="18.1">* Direct Impact</FOO> <FOO FN="18.2">** Reverse Impact</FOO> <FOO FN="18.3">*** Inch-Pounds</FOO> </TAB> Note :